Please copy and paste this embed script to where you want to embed

INTERNATIONAL INSTITUTE OF WELDING UNITED KINGDOM DELEGATION

Doc: IIW-XIII-WG1-114 - 03

Commission XIII - WG1

FEBRUARY 2003

BEST PRACTICE GUIDE ON STATISTICAL ANALYSIS OF FATIGUE DATA C R A Schneider and S J Maddox TWI, Granta Park, Great Abington, Cambridge, UK

1

TWI statistics report

CONTENTS GLOSSARY OF TERMS 1.

INTRODUCTION

1

2.

OBJECTIVE

1

3.

ASSUMPTIONS

1

3.1.

FORM OF S-N CURVE

1

3.2.

TESTS FOR LINEARITY OF RELATIONSHIP BETWEEN LOGS AND LOGN

2

3.3.

TESTS THAT N IS LOG-NORMALLY DISTRIBUTED

3

3.4.

TESTS OF HOMOGENEITY OF STANDARD DEVIATION OF LOGN WITH RESPECT TO S

3

3.5.

TESTS OF STATISTICAL INDEPENDENCE OF TEST RESULTS

3

4.

FITTING AN S-N CURVE

3

5.

TREATMENT OF RESULTS WHERE NO FAILURE HAS OCCURRED

4

5.1.

INTRODUCTION

4

5.2.

RESULTS ASSOCIATED WITH THE FATIGUE LIMIT

4

5.3. 5.3.1. 5.3.2.

FATIGUE TESTS STOPPED BEFORE FAILURE Maximum Likelihood Method Alternative Method based on Extreme Value Statistics

5 5 6

6.

ESTABLISHING A DESIGN (OR CHARACTERISTIC) CURVE

6

6.1.

PREDICTION LIMITS

6

6.2.

TOLERANCE LIMITS

7

6.3.

RESULTS WHERE NO FAILURE HAS OCCURRED

8

7.

PREDICTING FATIGUE LIFE

8

7.1.

INDIVIDUAL WELD

8

Copyright © 2003, The Welding Institute

7.2.

STRUCTURE CONTAINING MANY WELDS

8

8.

JUSTIFYING THE USE OF A GIVEN DESIGN CURVE FROM A NEW DATA SET

8

8.1.

PROBLEM

8

8.2.

APPROACH

9

8.3.

ASSUMPTIONS

9

8.4.

METHOD

10

8.5. 8.5.1. 8.5.2. 8.5.3.

PRACTICAL APPLICATIONS Tests Performed at the Same Stress Level Repeat Tests at Selected Stress Levels Tests Performed to Produce an S-N Curve

10 10 10 11

9.

TESTING WHETHER TWO DATA SETS ARE CONSISTENT

12

9.1.

PROBLEM

12

9.2.

APPROACH

12

9.3. 9.3.1. 9.3.2. 9.3.3.

TESTS PERFORMED AT THE SAME STRESS LEVEL General Test that Standard Deviations are Consistent Test that the Mean Fatigue Lives are Consistent

13 13 13 13

9.4. 9.4.1. 9.4.2. 9.4.3.

TESTS PERFORMED TO PRODUCE AN S-N CURVE Test that Residual Standard Deviations are Consistent Test that the Intercepts of the Two S-N Curves are Consistent Testing that the Slopes of the Two S-N curves are Consistent (t-test)

14 14 14 14

9.5.

COMPOSITE HYPOTHESES

14

10.

TESTING WHETHER MORE THAN TWO DATA SETS ARE CONSISTENT

15

10.1.

PROBLEM

15

10.2.

APPROACH

15

10.3. 10.3.1. 10.3.2. 10.3.3.

TESTS PERFORMED AT THE SAME STRESS LEVEL General Test that Standard Deviations are Consistent Test that Mean Fatigue Lives are Consistent

15 15 15 15

10.4. TESTS PERFORMED TO PRODUCE AN S-N CURVE 10.4.1. Test that Residual Standard Deviations are Consistent 10.4.2. Test that the Intercepts and Slopes of the S-N Curves are Consistent

Copyright © 2003, The Welding Institute

16 16 16

11.

SENSITIVITY OF DESIGN CURVE TO SAMPLE SIZE

16

12.

REFERENCES

17

TABLE 1 Appendix: Statistical Analysis of Fatigue Data obtained from Specimens Containing Many Welds

Copyright © 2003, The Welding Institute

GLOSSARY OF TERMS This glossary describes statistical terms as they are used in this guide, as well as those that are commonly used in other guidance documents/standards on this subject. Kendall and Buckland give more general definitions of these terms. Alternative hypothesis In decision theory, any admissible hypothesis that is distinct from the null hypothesis. Censored data Response data, such as fatigue endurance, is described as censored when its exact value is unknown but, for instance, it is known to fall within a certain range of values. Censored fatigue data is generally 'right' censored, which means that the endurance is known to be greater than a particular value (typically because the test stops before failure actually occurs). Characteristic curve/value A fatigue design (or characteristic) curve is established by adopting characteristic values that lie a certain number of standard deviations below the mean S-N curve (see Section 6). Chi-square distribution The chi-square, or χ2, distribution is the statistical distribution followed by the sum of squares of ν independent normal variates in standard form (i.e. having zero mean and standard deviation of one). It is useful in determining confidence limits for the standard deviation of a sample drawn from a normal distribution (see Section 8.3). Confidence interval/level /limits Confidence limits are statistics derived from sample values, between which a population parameter under estimation will lie with some fixed probability P% (called the confidence level). The interval between the upper and lower confidence limits is called a confidence interval. Degrees of freedom In regression analysis, the number of degrees of freedom f is equal to the sample size n minus the number of coefficients estimated by the regression. It is also used as a parameter of a number of distributions, including χ2, F and Student's t. Design curve See Characteristic curve. Extreme value statistic The statistic given by the smallest (or largest) observation in a sample. An extreme value statistic is a particular type of order statistic (so the terms are often used interchangeably). Gaussian distribution An alternative name for the normal distribution. Hypothesis Conjecture to be tested by some statistical analysis.

Copyright © 2003, The Welding Institute

Least squares method In regression analysis, a method of estimation in which the regression coefficients are estimated by minimising the sum of the squares of the deviations of the data points from the fitted regression line. In certain cases, the method is equivalent to the maximum likelihood method (see Section 5.3.1). Linear regression See regression. Log-normal distribution The distribution pertaining to the variate X when logX follows a normal distribution. Maximum likelihood method A method of estimating parameters of a population (e.g. regression coefficients) as those values for which the likelihood of obtaining the observed data is maximised (see Section 5.3.1). Normal distribution A symmetrical distribution that commonly arises as the sum of a large number of variates (e.g. measurement errors) having similar distributions to one another. For this reason, data is often assumed to follow a normal distribution in the absence of information to the contrary. Null hypothesis In decision theory, the hypothesis under test. Order statistics When a sample is arranged in ascending order of magnitude, the ordered values are called order statistics. The term can also refer, more specifically, to the extreme values of the sample. Population The complete set from which a random sample is taken, e.g. the set of S-N data from all components of a given type, in the context of fatigue testing. Prediction interval/limits Prediction limits are the limits between which a given proportion (typically 95%) of the population lies. The interval between the upper and lower prediction limits is called a prediction interval. Random variable See variate. Regression Process of estimating the coefficients of an equation for predicting a response y (such as logN) in terms of certain independent variates (such as logS). In the case of linear regression, the fitted equation is of the form y = mx + c. Significance level In decision theory, the probability (typically set to 5%) that the null hypothesis will be incorrectly rejected when it is, in fact, true. 13604.01/02/1157.02 Copyright © 2002, The Welding Institute

Standard deviation The most widely used measure of dispersion of a variate, equal to the square root of the variance. Student's t distribution The t distribution is the statistical distribution of the ratio of a sample mean to a sample variance for samples from a normal distribution in standard form (i.e. having zero mean and standard deviation of one). It is useful in determining confidence limits for the mean of a small sample drawn from a normal distribution. Tolerance limits Tolerance limits are values of a variate, following a given type of distribution, between which it is stated with confidence γ % that at least a proportion P% of the population will lie. This statement is made on the basis of a sample of n independent observations. A tolerance limit can thus regarded to be a confidence limit on a confidence limit. Variance The mean of the squared deviations of a variate from its arithmetic mean. Variate A quantity (also called random variable) that may take any of the values of a specified set with a specified relative frequency or probability.

13604.01/02/1157.02 Copyright © 2002, The Welding Institute

1.

INTRODUCTION

Fatigue testing is the main basis of the relationship between the fatigue resistance of a given material, component or structural detail and cyclic loading. The results of such fatigue endurance tests are plotted on graphs relating applied loading (force, stress, strain, etc) and the number of cycles to failure. Since test specimens and testing conditions are never identical, the resulting data are invariably scattered. Consequently, some judgement is required when using them to establish the required relationship. Statistical methods are available to assist in this analysis of fatigue test data, and indeed some recommendations on their use for analysing fatigue data are available.1,2 However, they do not deal with all the statistical analyses that may be required to utilise fatigue test results and none of them offers specific guidelines for analysing fatigue data obtained from tests on welded specimens. With the increasing use of fatigue testing to supplement design rules, an approach that is now encouraged in some Standards3-5, there is a need for comprehensive guidance on the statistical analysis of fatigue test results. This is the subject of the present Best Practice Guide. At this stage, the focus is on fatigue endurance test results obtained under constant amplitude loading, as used to produce S-N curves. Thus, the loading is expressed as a stress range, S, and the fatigue resistance is expressed as the number of cycles, N, that can be endured by the test specimen. In general, however, the same methods can be applied to fatigue endurance test results expressed using any measure of the loading (e.g. force, strain) and results obtained under variable amplitude loading. They can also be used to analyse fatigue crack propagation data, where the loading is expressed as the stress intensity factor range, ∆K, and the fatigue resistance is expressed as the rate of crack propagation da/dN. Since the analyses are concerned purely with the experimental data, they are independent of the material tested. 2. •

OBJECTIVE To establish best practice for the statistical analysis of fatigue data obtained from welded specimens.

3.

ASSUMPTIONS

3.1.

FORM OF S-N CURVE

a) There is an underlying linear relationship between logS and logN of the form:

log N

=

log A − m log S

[1]

where m is the slope and log A is the intercept. This can be re-written in a form that is commonly used to describe S-N curves in design rules: Sm N = A

[2]

Note that, in practice, this assumption will only hold true between certain limits on S, as illustrated in Fig. 1. The lower limit on S is determined by the fatigue endurance limit (or just 'fatigue limit'), the stress range below which fatigue failure will not occur. In practice this is usually chosen on the basis of the endurance that can be achieved without any evidence of fatigue cracking, typically between N = 2 × 106 and 107 cycles. The upper limit on S is dependent on the static strength of the test specimen but is commonly taken to be the 1 13604.01/02/1157.02 Copyright © 2002, The Welding Institute

maximum allowable static design stress6. However, the linear relationship between applied strain range and fatigue life for data obtained under strain control extends to much higher pseudo-elastic stress (i.e. strain × elastic modulus) levels. b) The fatigue life N for a given stress range S is log-normally distributed. c) The standard deviation of log N does not vary with S. d) Each test result is statistically independent of the others. These assumptions are rarely challenged in practice. But, if there is any reason to doubt their validity, there are statistical tests available that can help to identify departures from these assumptions. Some of these tests are listed below.

500 Test result Ò Specimen unfailed

300

M aximum applie d stre ss approaching static stre ngth

2

m 200 m / N , e g n 100 ar s s er t S 50

Applie d stre ss range approaching fatigue limit

Range ov e r which data can be use d to e stimate be st-fit line ar S-N curv e

30 3

10

4

5

10

10

6

10

7

10

Endurance, cycles

Fig.1 Typical fatigue endurance test data illustrating deviations from linear S-N curve. 3.2.

TESTS FOR LINEARITY OF RELATIONSHIP BETWEEN LOGS AND LOGN

One common method of testing for non-linearity in a relationship is to fit a polynomial (typically a quadratic or cubic) in logS to the data. Polynomial regression is available within most statistical software packages (e.g. MINITAB7). Analysis of Variance (ANOVA) can then be used to test whether the quadratic/cubic regression components are statistically significant (see Ferguson8 for a worked example).

2 13604.01/02/1157.02 Copyright © 2002, The Welding Institute

Box and Tidwell9 describe a less well-known approach, which is to add a term of the form (logS)ln(logS) to the usual linear regression model. If the coefficient in this variable is significant, then this can be taken as evidence of non-linearity. 3.3.

TESTS THAT N IS LOG-NORMALLY DISTRIBUTED

The simplest check is an 'eyeball' assessment of whether a normal probability plot of the departures (or 'residuals') of logN from the regression line of logS versus logN follows a linear trend. This can be done either by using standard statistical software, or by plotting the residuals on normal probability paper. There is also a wide variety of formal statistic-based tests of normality, many of which are implemented in statistical software packages.10-14 3.4.

TESTS OF TO S

HOMOGENEITY

OF

STANDARD DEVIATION

OF

LOGN

WITH

RESPECT

This assumption is most easily checked by simply examining a plot of the 'residuals' from the regression versus logS. The assessment can be backed up by partitioning the residuals into appropriate groups and applying either Bartlett's test,15 if logN is believed to be normally distributed, or otherwise Levene's test.7 3.5.

TESTS OF STATISTICAL INDEPENDENCE OF TEST RESULTS

This assumption is difficult to check, in practice. A good starting point is to examine plots of the 'residuals' from the regression against both logS and against the order in which the results were collected (in case there is some time-dependence). There should not be any recognisable patterns in the residuals in either of these plots. If there are, the data can be grouped accordingly, and variations in the mean level can then be tested using Analysis of Variance. Any inhomogeneity in the standard deviations of the groups can be tested as in Section 3.4. 4.

FITTING AN S-N CURVE

In their simplest form, S-N data comprise n data points (logSi, logNi), where Si is the stress range and Ni is the endurance in cycles. This endurance is either the number of cycles to failure (or some pre-determined criterion, such as the attainment of a particular size of fatigue crack) or the number of cycles endured without failure. Fig.2 shows an example of such data, together with some fitted S-N curves.16 Special attention is drawn to the fact that fatigue test results are traditionally plotted with logS as the y-axis and logN as the x-axis. The standard approach in curve fitting is to assume that the parameter plotted on the x-axis is the independent variable and that plotted on the y-axis is the dependent variable. However, the opposite is the case with fatigue data presented in the traditional way. Consequently, care is needed to ensure that logN is treated as the dependent variable. Considering only the results from specimens that failed, the intercept logA and slope m of the 'best fit' line through the data (called the 'mean' line in Fig.2) are estimated by ordinary linear regression, as described by Gurney and Maddox.6. The method usually used to estimate the slope and intercept coefficients is called 'least squares estimation'. This method is based on choosing those values of the coefficients that minimise the sum of the squared deviations (or 'residuals') of the observed values of log Ni from those predicted by the fitted line. TWI 3 13604.01/02/1157.02 Copyright © 2002, The Welding Institute

originally used such data and this method of analysis to derive the fatigue design rules for welded steel structures that have since formed the basis of most fatigue design rules in the world6,17.

350 300

T

R = 0.1

250

2

m m / N , e g n ar s s er t S

200

L

Structural steel T = 13mm L/T = 2.2 - 2.6

150

100 Ò

Results Specim en unfailed Mean and m ean ± 2 standard deviations of log N (95% confidence intervals) fitted to results from failed specim ens only

60 4

5x10

5

6

10

10

7

10

7

2x10

Endurance, cycles

Fig.2 Example of S-N data (Maddox)16 5.

TREATMENT OF RESULTS WHERE NO FAILURE HAS OCCURRED

5.1.

INTRODUCTION

In Section 4, it was assumed that each specimen under test yielded an exact failure endurance. However, there are circumstances in which results are obtained from specimens, or parts of specimens, that have not failed. Such results, which are plotted in Fig.1 and 2 as 'Specimen unfailed', are often termed 'run-outs'. Depending on the circumstances, it may or may not be possible to use the results from unfailed specimens in the statistical analysis of the data. Indeed, even nearby results from specimens that did fail may need to be excluded from that analysis. 5.2.

RESULTS ASSOCIATED WITH THE FATIGUE LIMIT

Most components exhibit a fatigue endurance limit under constant amplitude loading, defined as the stress range below which failure will not occur. In order to establish the constant amplitude fatigue limit (CAFL) experimentally, it is generally assumed to be the highest applied stress range for a given applied mean stress or stress ratio (minimum/maximum applied stress) at and below which the test specimen endures a particular number of cycles without showing any evidence of fatigue cracking. In smooth specimens, with no obvious stress concentration features, that endurance is usually around 2 x 106 cycles. However, in severely notched components, including most weld details, 107 cycles is commonly chosen. 4 13604.01/02/1157.02 Copyright © 2002, The Welding Institute

For design purposes, it is usually assumed that the S-N curve extends down to the CAFL and then turns sharply to become a horizontal line. The data in Fig.2 have been treated in this way, with the assumption that the CAFL coincides with N = 5 x 106 cycles in this case, as assumed in some fatigue design rules17. However, in practice fatigue test results usually follow an S-N curve that gradually changes slope in the region of the CAFL, as illustrated in Fig.1. Clearly, test results from either failed or unfailed specimens that lie in this transition region approaching the CAFL should not be combined with those obtained at higher stresses when estimating the best-fit linear S-N curve. Some judgement is needed when deciding which results fall into this category but, as a guide, any from notched or welded specimens that give N < 2 x 106 cycles could be included, or N

View more...
Doc: IIW-XIII-WG1-114 - 03

Commission XIII - WG1

FEBRUARY 2003

BEST PRACTICE GUIDE ON STATISTICAL ANALYSIS OF FATIGUE DATA C R A Schneider and S J Maddox TWI, Granta Park, Great Abington, Cambridge, UK

1

TWI statistics report

CONTENTS GLOSSARY OF TERMS 1.

INTRODUCTION

1

2.

OBJECTIVE

1

3.

ASSUMPTIONS

1

3.1.

FORM OF S-N CURVE

1

3.2.

TESTS FOR LINEARITY OF RELATIONSHIP BETWEEN LOGS AND LOGN

2

3.3.

TESTS THAT N IS LOG-NORMALLY DISTRIBUTED

3

3.4.

TESTS OF HOMOGENEITY OF STANDARD DEVIATION OF LOGN WITH RESPECT TO S

3

3.5.

TESTS OF STATISTICAL INDEPENDENCE OF TEST RESULTS

3

4.

FITTING AN S-N CURVE

3

5.

TREATMENT OF RESULTS WHERE NO FAILURE HAS OCCURRED

4

5.1.

INTRODUCTION

4

5.2.

RESULTS ASSOCIATED WITH THE FATIGUE LIMIT

4

5.3. 5.3.1. 5.3.2.

FATIGUE TESTS STOPPED BEFORE FAILURE Maximum Likelihood Method Alternative Method based on Extreme Value Statistics

5 5 6

6.

ESTABLISHING A DESIGN (OR CHARACTERISTIC) CURVE

6

6.1.

PREDICTION LIMITS

6

6.2.

TOLERANCE LIMITS

7

6.3.

RESULTS WHERE NO FAILURE HAS OCCURRED

8

7.

PREDICTING FATIGUE LIFE

8

7.1.

INDIVIDUAL WELD

8

Copyright © 2003, The Welding Institute

7.2.

STRUCTURE CONTAINING MANY WELDS

8

8.

JUSTIFYING THE USE OF A GIVEN DESIGN CURVE FROM A NEW DATA SET

8

8.1.

PROBLEM

8

8.2.

APPROACH

9

8.3.

ASSUMPTIONS

9

8.4.

METHOD

10

8.5. 8.5.1. 8.5.2. 8.5.3.

PRACTICAL APPLICATIONS Tests Performed at the Same Stress Level Repeat Tests at Selected Stress Levels Tests Performed to Produce an S-N Curve

10 10 10 11

9.

TESTING WHETHER TWO DATA SETS ARE CONSISTENT

12

9.1.

PROBLEM

12

9.2.

APPROACH

12

9.3. 9.3.1. 9.3.2. 9.3.3.

TESTS PERFORMED AT THE SAME STRESS LEVEL General Test that Standard Deviations are Consistent Test that the Mean Fatigue Lives are Consistent

13 13 13 13

9.4. 9.4.1. 9.4.2. 9.4.3.

TESTS PERFORMED TO PRODUCE AN S-N CURVE Test that Residual Standard Deviations are Consistent Test that the Intercepts of the Two S-N Curves are Consistent Testing that the Slopes of the Two S-N curves are Consistent (t-test)

14 14 14 14

9.5.

COMPOSITE HYPOTHESES

14

10.

TESTING WHETHER MORE THAN TWO DATA SETS ARE CONSISTENT

15

10.1.

PROBLEM

15

10.2.

APPROACH

15

10.3. 10.3.1. 10.3.2. 10.3.3.

TESTS PERFORMED AT THE SAME STRESS LEVEL General Test that Standard Deviations are Consistent Test that Mean Fatigue Lives are Consistent

15 15 15 15

10.4. TESTS PERFORMED TO PRODUCE AN S-N CURVE 10.4.1. Test that Residual Standard Deviations are Consistent 10.4.2. Test that the Intercepts and Slopes of the S-N Curves are Consistent

Copyright © 2003, The Welding Institute

16 16 16

11.

SENSITIVITY OF DESIGN CURVE TO SAMPLE SIZE

16

12.

REFERENCES

17

TABLE 1 Appendix: Statistical Analysis of Fatigue Data obtained from Specimens Containing Many Welds

Copyright © 2003, The Welding Institute

GLOSSARY OF TERMS This glossary describes statistical terms as they are used in this guide, as well as those that are commonly used in other guidance documents/standards on this subject. Kendall and Buckland give more general definitions of these terms. Alternative hypothesis In decision theory, any admissible hypothesis that is distinct from the null hypothesis. Censored data Response data, such as fatigue endurance, is described as censored when its exact value is unknown but, for instance, it is known to fall within a certain range of values. Censored fatigue data is generally 'right' censored, which means that the endurance is known to be greater than a particular value (typically because the test stops before failure actually occurs). Characteristic curve/value A fatigue design (or characteristic) curve is established by adopting characteristic values that lie a certain number of standard deviations below the mean S-N curve (see Section 6). Chi-square distribution The chi-square, or χ2, distribution is the statistical distribution followed by the sum of squares of ν independent normal variates in standard form (i.e. having zero mean and standard deviation of one). It is useful in determining confidence limits for the standard deviation of a sample drawn from a normal distribution (see Section 8.3). Confidence interval/level /limits Confidence limits are statistics derived from sample values, between which a population parameter under estimation will lie with some fixed probability P% (called the confidence level). The interval between the upper and lower confidence limits is called a confidence interval. Degrees of freedom In regression analysis, the number of degrees of freedom f is equal to the sample size n minus the number of coefficients estimated by the regression. It is also used as a parameter of a number of distributions, including χ2, F and Student's t. Design curve See Characteristic curve. Extreme value statistic The statistic given by the smallest (or largest) observation in a sample. An extreme value statistic is a particular type of order statistic (so the terms are often used interchangeably). Gaussian distribution An alternative name for the normal distribution. Hypothesis Conjecture to be tested by some statistical analysis.

Copyright © 2003, The Welding Institute

Least squares method In regression analysis, a method of estimation in which the regression coefficients are estimated by minimising the sum of the squares of the deviations of the data points from the fitted regression line. In certain cases, the method is equivalent to the maximum likelihood method (see Section 5.3.1). Linear regression See regression. Log-normal distribution The distribution pertaining to the variate X when logX follows a normal distribution. Maximum likelihood method A method of estimating parameters of a population (e.g. regression coefficients) as those values for which the likelihood of obtaining the observed data is maximised (see Section 5.3.1). Normal distribution A symmetrical distribution that commonly arises as the sum of a large number of variates (e.g. measurement errors) having similar distributions to one another. For this reason, data is often assumed to follow a normal distribution in the absence of information to the contrary. Null hypothesis In decision theory, the hypothesis under test. Order statistics When a sample is arranged in ascending order of magnitude, the ordered values are called order statistics. The term can also refer, more specifically, to the extreme values of the sample. Population The complete set from which a random sample is taken, e.g. the set of S-N data from all components of a given type, in the context of fatigue testing. Prediction interval/limits Prediction limits are the limits between which a given proportion (typically 95%) of the population lies. The interval between the upper and lower prediction limits is called a prediction interval. Random variable See variate. Regression Process of estimating the coefficients of an equation for predicting a response y (such as logN) in terms of certain independent variates (such as logS). In the case of linear regression, the fitted equation is of the form y = mx + c. Significance level In decision theory, the probability (typically set to 5%) that the null hypothesis will be incorrectly rejected when it is, in fact, true. 13604.01/02/1157.02 Copyright © 2002, The Welding Institute

Standard deviation The most widely used measure of dispersion of a variate, equal to the square root of the variance. Student's t distribution The t distribution is the statistical distribution of the ratio of a sample mean to a sample variance for samples from a normal distribution in standard form (i.e. having zero mean and standard deviation of one). It is useful in determining confidence limits for the mean of a small sample drawn from a normal distribution. Tolerance limits Tolerance limits are values of a variate, following a given type of distribution, between which it is stated with confidence γ % that at least a proportion P% of the population will lie. This statement is made on the basis of a sample of n independent observations. A tolerance limit can thus regarded to be a confidence limit on a confidence limit. Variance The mean of the squared deviations of a variate from its arithmetic mean. Variate A quantity (also called random variable) that may take any of the values of a specified set with a specified relative frequency or probability.

13604.01/02/1157.02 Copyright © 2002, The Welding Institute

1.

INTRODUCTION

Fatigue testing is the main basis of the relationship between the fatigue resistance of a given material, component or structural detail and cyclic loading. The results of such fatigue endurance tests are plotted on graphs relating applied loading (force, stress, strain, etc) and the number of cycles to failure. Since test specimens and testing conditions are never identical, the resulting data are invariably scattered. Consequently, some judgement is required when using them to establish the required relationship. Statistical methods are available to assist in this analysis of fatigue test data, and indeed some recommendations on their use for analysing fatigue data are available.1,2 However, they do not deal with all the statistical analyses that may be required to utilise fatigue test results and none of them offers specific guidelines for analysing fatigue data obtained from tests on welded specimens. With the increasing use of fatigue testing to supplement design rules, an approach that is now encouraged in some Standards3-5, there is a need for comprehensive guidance on the statistical analysis of fatigue test results. This is the subject of the present Best Practice Guide. At this stage, the focus is on fatigue endurance test results obtained under constant amplitude loading, as used to produce S-N curves. Thus, the loading is expressed as a stress range, S, and the fatigue resistance is expressed as the number of cycles, N, that can be endured by the test specimen. In general, however, the same methods can be applied to fatigue endurance test results expressed using any measure of the loading (e.g. force, strain) and results obtained under variable amplitude loading. They can also be used to analyse fatigue crack propagation data, where the loading is expressed as the stress intensity factor range, ∆K, and the fatigue resistance is expressed as the rate of crack propagation da/dN. Since the analyses are concerned purely with the experimental data, they are independent of the material tested. 2. •

OBJECTIVE To establish best practice for the statistical analysis of fatigue data obtained from welded specimens.

3.

ASSUMPTIONS

3.1.

FORM OF S-N CURVE

a) There is an underlying linear relationship between logS and logN of the form:

log N

=

log A − m log S

[1]

where m is the slope and log A is the intercept. This can be re-written in a form that is commonly used to describe S-N curves in design rules: Sm N = A

[2]

Note that, in practice, this assumption will only hold true between certain limits on S, as illustrated in Fig. 1. The lower limit on S is determined by the fatigue endurance limit (or just 'fatigue limit'), the stress range below which fatigue failure will not occur. In practice this is usually chosen on the basis of the endurance that can be achieved without any evidence of fatigue cracking, typically between N = 2 × 106 and 107 cycles. The upper limit on S is dependent on the static strength of the test specimen but is commonly taken to be the 1 13604.01/02/1157.02 Copyright © 2002, The Welding Institute

maximum allowable static design stress6. However, the linear relationship between applied strain range and fatigue life for data obtained under strain control extends to much higher pseudo-elastic stress (i.e. strain × elastic modulus) levels. b) The fatigue life N for a given stress range S is log-normally distributed. c) The standard deviation of log N does not vary with S. d) Each test result is statistically independent of the others. These assumptions are rarely challenged in practice. But, if there is any reason to doubt their validity, there are statistical tests available that can help to identify departures from these assumptions. Some of these tests are listed below.

500 Test result Ò Specimen unfailed

300

M aximum applie d stre ss approaching static stre ngth

2

m 200 m / N , e g n 100 ar s s er t S 50

Applie d stre ss range approaching fatigue limit

Range ov e r which data can be use d to e stimate be st-fit line ar S-N curv e

30 3

10

4

5

10

10

6

10

7

10

Endurance, cycles

Fig.1 Typical fatigue endurance test data illustrating deviations from linear S-N curve. 3.2.

TESTS FOR LINEARITY OF RELATIONSHIP BETWEEN LOGS AND LOGN

One common method of testing for non-linearity in a relationship is to fit a polynomial (typically a quadratic or cubic) in logS to the data. Polynomial regression is available within most statistical software packages (e.g. MINITAB7). Analysis of Variance (ANOVA) can then be used to test whether the quadratic/cubic regression components are statistically significant (see Ferguson8 for a worked example).

2 13604.01/02/1157.02 Copyright © 2002, The Welding Institute

Box and Tidwell9 describe a less well-known approach, which is to add a term of the form (logS)ln(logS) to the usual linear regression model. If the coefficient in this variable is significant, then this can be taken as evidence of non-linearity. 3.3.

TESTS THAT N IS LOG-NORMALLY DISTRIBUTED

The simplest check is an 'eyeball' assessment of whether a normal probability plot of the departures (or 'residuals') of logN from the regression line of logS versus logN follows a linear trend. This can be done either by using standard statistical software, or by plotting the residuals on normal probability paper. There is also a wide variety of formal statistic-based tests of normality, many of which are implemented in statistical software packages.10-14 3.4.

TESTS OF TO S

HOMOGENEITY

OF

STANDARD DEVIATION

OF

LOGN

WITH

RESPECT

This assumption is most easily checked by simply examining a plot of the 'residuals' from the regression versus logS. The assessment can be backed up by partitioning the residuals into appropriate groups and applying either Bartlett's test,15 if logN is believed to be normally distributed, or otherwise Levene's test.7 3.5.

TESTS OF STATISTICAL INDEPENDENCE OF TEST RESULTS

This assumption is difficult to check, in practice. A good starting point is to examine plots of the 'residuals' from the regression against both logS and against the order in which the results were collected (in case there is some time-dependence). There should not be any recognisable patterns in the residuals in either of these plots. If there are, the data can be grouped accordingly, and variations in the mean level can then be tested using Analysis of Variance. Any inhomogeneity in the standard deviations of the groups can be tested as in Section 3.4. 4.

FITTING AN S-N CURVE

In their simplest form, S-N data comprise n data points (logSi, logNi), where Si is the stress range and Ni is the endurance in cycles. This endurance is either the number of cycles to failure (or some pre-determined criterion, such as the attainment of a particular size of fatigue crack) or the number of cycles endured without failure. Fig.2 shows an example of such data, together with some fitted S-N curves.16 Special attention is drawn to the fact that fatigue test results are traditionally plotted with logS as the y-axis and logN as the x-axis. The standard approach in curve fitting is to assume that the parameter plotted on the x-axis is the independent variable and that plotted on the y-axis is the dependent variable. However, the opposite is the case with fatigue data presented in the traditional way. Consequently, care is needed to ensure that logN is treated as the dependent variable. Considering only the results from specimens that failed, the intercept logA and slope m of the 'best fit' line through the data (called the 'mean' line in Fig.2) are estimated by ordinary linear regression, as described by Gurney and Maddox.6. The method usually used to estimate the slope and intercept coefficients is called 'least squares estimation'. This method is based on choosing those values of the coefficients that minimise the sum of the squared deviations (or 'residuals') of the observed values of log Ni from those predicted by the fitted line. TWI 3 13604.01/02/1157.02 Copyright © 2002, The Welding Institute

originally used such data and this method of analysis to derive the fatigue design rules for welded steel structures that have since formed the basis of most fatigue design rules in the world6,17.

350 300

T

R = 0.1

250

2

m m / N , e g n ar s s er t S

200

L

Structural steel T = 13mm L/T = 2.2 - 2.6

150

100 Ò

Results Specim en unfailed Mean and m ean ± 2 standard deviations of log N (95% confidence intervals) fitted to results from failed specim ens only

60 4

5x10

5

6

10

10

7

10

7

2x10

Endurance, cycles

Fig.2 Example of S-N data (Maddox)16 5.

TREATMENT OF RESULTS WHERE NO FAILURE HAS OCCURRED

5.1.

INTRODUCTION

In Section 4, it was assumed that each specimen under test yielded an exact failure endurance. However, there are circumstances in which results are obtained from specimens, or parts of specimens, that have not failed. Such results, which are plotted in Fig.1 and 2 as 'Specimen unfailed', are often termed 'run-outs'. Depending on the circumstances, it may or may not be possible to use the results from unfailed specimens in the statistical analysis of the data. Indeed, even nearby results from specimens that did fail may need to be excluded from that analysis. 5.2.

RESULTS ASSOCIATED WITH THE FATIGUE LIMIT

Most components exhibit a fatigue endurance limit under constant amplitude loading, defined as the stress range below which failure will not occur. In order to establish the constant amplitude fatigue limit (CAFL) experimentally, it is generally assumed to be the highest applied stress range for a given applied mean stress or stress ratio (minimum/maximum applied stress) at and below which the test specimen endures a particular number of cycles without showing any evidence of fatigue cracking. In smooth specimens, with no obvious stress concentration features, that endurance is usually around 2 x 106 cycles. However, in severely notched components, including most weld details, 107 cycles is commonly chosen. 4 13604.01/02/1157.02 Copyright © 2002, The Welding Institute

For design purposes, it is usually assumed that the S-N curve extends down to the CAFL and then turns sharply to become a horizontal line. The data in Fig.2 have been treated in this way, with the assumption that the CAFL coincides with N = 5 x 106 cycles in this case, as assumed in some fatigue design rules17. However, in practice fatigue test results usually follow an S-N curve that gradually changes slope in the region of the CAFL, as illustrated in Fig.1. Clearly, test results from either failed or unfailed specimens that lie in this transition region approaching the CAFL should not be combined with those obtained at higher stresses when estimating the best-fit linear S-N curve. Some judgement is needed when deciding which results fall into this category but, as a guide, any from notched or welded specimens that give N < 2 x 106 cycles could be included, or N

Thank you for interesting in our services. We are a non-profit group that run this website to share documents. We need your help to maintenance this website.

To keep our site running, we need your help to cover our server cost (about $400/m), a small donation will help us a lot.